Polyamide 66 microspheres metallised with in situ synthesised gold nanoparticles for a catalytic application
© Cheval et al; licensee Springer. 2012
Received: 24 August 2011
Accepted: 8 March 2012
Published: 8 March 2012
A simple concept is proposed to metallise polyamide 66 (PA66) spherulite structures with in situ synthesised gold nanoparticles (Au NPs) using a wet chemical method. This cost-effective approach, applied to produce a PA66/Au NP hybrid material, offers the advantages of controlling the nanoparticle size, the size distribution and the organic-inorganic interactions. These are the key factors that have to be controlled to construct consistent Au nanostructures which are essential for producing the catalytic activities of interest. The hybrid materials obtained are characterised by means of scanning electron microscopy, transmission electron microscopy, attenuated total reflection-Fourier transform infrared spectrometry and X-ray diffraction spectrometry. The results show that PA66 microspheres obtained via the crystallisation process are coated with Au NPs of 13 nm in size. It was found that controlling the metal coordination is the key parameter to template the Au NPs on the spherulite surfaces. The preparation processes and the key factors leading to the formation of PA66 spherulites coated with Au NPs are discussed. Moreover, the efficiency of the coated spherulites as a potential catalyst is proved by demonstrating the reduction of methylene blue via UV-visible spectrometry.
Keywordspolyamide 66 nanoparticle catalyst microsphere gold spherulites
Immobilising noble metal nanoparticles onto organic microsphere surface has been receiving a considerable amount of attention in chemical fields due to their interesting catalytic properties and useful practical applications [1–3]. Additionally, organic microspheres offer the advantage to be easily recycled by conventional filtration or centrifugation techniques [4–6]. Furthermore, it has been found that this spherical structure is an excellent support for promoting the intriguing catalytic properties of noble metal nanoparticles [7–9].
Over the last few years, various organic supports have been utilised to stabilise metallic nanoparticles [7–9]. For instance, Dokoutchaev et al. reported the fabrication of polystyrene (PS) microspheres coated with Au, Pt and Pd nanoparticles . Whereas, Jeon et al. synthesised hierarchically structured microspheres composed of a PS-b-PEO diblock copolymer and gold nanoparticles . These hybrid systems possess weak mechanical properties and low catalytic activities and are often complex to produce .
Controlling the nanoparticle diameter is found to be the key factor for harnessing their catalytic properties. Indeed, gold and palladium in bulk state are chemically inert but become chemically active for many reactions at a nanoscale level. It has been found that decreasing the particle size to nanoscale decreases their redox potential to a negative value [15–19]. Due to their high specific surface area and their low redox potential, stabilised noble metal nanoparticles are usually used in the chemical field as an effective catalyst [5, 12].
Herein, we propose a simple concept to coat PA66 spherulites with gold nanoparticles (Au NPs) prepared in situ via a wet chemical approach. This cost-effective method offers the advantages of controlling the particle size, the size distribution and also the organic-inorganic interactions .
PA66/Au NP hybrid materials obtained were characterised by scanning electron microscopy (SEM), transmission electron microscopy (TEM), attenuated total reflection-Fourier transform infrared spectrometry (ATR-FTIR), energy-dispersive X-ray (EDX) analysis and X-ray diffraction (XRD) spectrometry. The catalytic property of PA66/Au NP microspheres was tested by investigating the reduction of methylene blue to leuco methylene blue in water medium using UV-visible (UV-Vis) spectrometry.
Commercial PA66 (Mw = 18,000 mg/ml) in pellet forms was supplied by Celanese Chemicals UK Ltd. (Stallingborough, UK). Gold chloride (HAuCl4), formic acid (HCOOH) and sodium borohydride (NaBH4) were purchased from Sigma-Aldrich Company Ltd. (Dorset, England, UK) and used as received.
PA66 spherulite preparation
PA66 in a pellet form was dissolved in 98% formic acid. Distilled water was added slowly into the PA66 solution to crystallise the polymer in order to form spherulites (Figure 1). The powder recovered was dried for 3 h at 110°C. The PA66 average spherulite diameter size determined by dynamic light scattering (DLS) was estimated at 179.4 nm [see Additional file 1].
Metallisation of PA66 spherulites
The PA66 powder recovered from the spherulite preparation process was mixed with the gold precursor (HAuCl4) solution in water. The mixture was stirred for 24 h to ensure the coordination between the organic and inorganic materials. The PA66/HAuCl4 system was then centrifuged and rinsed a few times to remove the excess of gold chloride. The system was re-dispersed in aqueous medium, and sodium borohydride was incorporated into the solution to reduce the gold precursor into Au NPs. Finally, the PA66/Au NP hybrid material powder was washed with distilled water to remove NaBH4 compound and subsequently dried at 110°C for 3 h to remove excess water.
Pristine and metallised PA66 spherulites were observed with a scanning electron microscope (model XL 30 ESEM FEG, Philips, Guildford, England, UK). PA66/Au NP microspheres were not coated to avoid the overlapping with the metal-conducting layer. EDX analysis was carried out on the sample at a working distance of 10 mm, using the INCA software (Oxford Instruments, Abingdon, UK). To assess the particle size and size distribution, the specimen was observed via a transmission electron microscope at 100 keV (Tecnai BioTWIN, FEI Ltd., Hillsboro, OR, USA). The TEM micrographs obtained were analysed with the program Gwyddion using the grain analysis function. UV-Vis spectra were recorded using a Varian Cary 50 photospectrometer (Varian Medical Systems UK Ltd., Crawley, UK) with the monochromator slit width of 10 nm. To determine the type of interaction between Au NPs and PA66, ATR-FTIR (Tensor 27, Bruker Optics, Rheinstetten, Germany) measurements were conducted at ambient temperature in the spectral range from 4,000 to 550 cm-1 on the PA66/Au NP hybrid material powder recovered.
Reduction of MB
A solution of methylene blue (MB) was prepared in aqueous medium at 1 mg/ml. One milligram of sodium borohydride (NaBH4) was added to 1 ml of MB solution. Optical absorption spectrum of the solution was measured every 4 min after the incorporation of NaBH4 by UV-Vis spectrometry. One milligram of the PA66/Au NP microsphere powder was added to the MB-NaBH4 solution. Then, the optical absorption spectrum of the solution was also recorded every 4 min to investigate the reduction of MB in the presence of PA66/Au microspheres.
Results and discussion
Characteristic vibrations of PA66 and PA66 coated with Au NPs
PA66 coated with Au NPs (cm-1)
N-H Stretching vibration
N-H Bending vibration
C = O Stretching vibration
N-H Bending vibration
-CH2- Stretching vibration
In chemistry, this substance is recognised as a redox indicator since it can easily change its colour in a specific environment [4, 24]. Indeed, MB, initially blue in an oxidizing environment, undergoes a definite colour change by becoming colourless in the presence of a reducing agent such as sodium borohydride . The MB reduction reaction, leading to the formation of LMB, is described in Figure 7.
In aqueous medium, MB exhibits a main absorption peak at 664 nm with a shoulder at 614 nm as shown in Figure 8. It has been reported that the main absorption peak at 664 nm corresponds to the n-π* transition of MB [26, 27]. The reduction of MB as a function of time has been investigated in the presence of sodium borohydride. Relative absorbance of the peak at 664 nm is plotted as a function of time to evaluate the MB reduction reaction rate (Figure 8b). Incorporation of the reducing agent into the MB solution decreases slightly the absorbance intensity of the peak at 664 nm with the time (Figure 8b, see Additional file 2). This decreasing trend indicates that MB starts to reduce in the presence of NaBH4; however, the reaction is slow. After 20 min, the PA66/Au NP hybrid system was incorporated into the MB/NaBH4 solution. Interestingly, a strong decrease of the UV-Vis absorbance intensity of MB is observed in the presence of the hybrid material (Figure 8a, b). Additionally, the plot of the relative absorbance of the peak at 664 nm reveals that the complete reduction of MB to LMB is accomplished in less than 20 min in the presence of the hybrid materials since the curve tends to stabilise at the end (Figure 8b). This result confirms that PA66/Au NP hybrid microspheres act as an effective catalyst in the reduction of MB.
To summarise, a simple concept is applied to coat PA66 spherulites with Au NPs using a wet chemical method. The acidification of the solution due to the gold chloride dissociation results in the protonation of the amine group at the edge of the PA66 spherulites which favour the coordination with gold complex charged negatively. After reduction of the gold precursor, Au NPs covered the PA66 microsphere surfaces due to the physical interaction formed between both materials. PA66/Au NP hybrid material shows interesting catalytic activities. It has been found that Au NPs coated onto the PA66 spherulite act as an electron relay in the MB reduction since the redox potential of Au NPs produced is higher than the donor potential (E°(B2H4/BH4-)), but lower than the acceptor potential (E°(LMB/MB)). This approach could be applied to fabricate a variety of hybrid microspheres based on PA66 spherulites and different types of metallic nanoparticles for a wide range of catalytic and chemical applications.
This work was funded by the UK Engineering and Physical Science Research Council (EPSRC) through their Nottingham Innovation Research Centre.
- Caruso F, Spasova M, Salgueiriño-Maceira V, Liz-Marzán LM: Multilayer assemblies of silica-encapsulated gold nanoparticles on decomposable colloid templates. Adv Mater 2001, 13: 1090–1094. 10.1002/1521-4095(200107)13:14<1090::AID-ADMA1090>3.0.CO;2-HView ArticleGoogle Scholar
- Li S, Yang X, Huang W: Synthesis of monodisperse polymer microspheres with mercapto groups and their application as a stabilizer for gold metallic colloid. Macromol Chem Physic 2005, 206: 1967–1672. 10.1002/macp.200500216View ArticleGoogle Scholar
- Walsh D, Mann S: Fabrication of hollow porous shells of calcium carbonate from self-organizing media. Nature 1995, 377: 320–323. 10.1038/377320a0View ArticleGoogle Scholar
- Cheng X, Tjong SIEC, Zhao Q, Li RKY: Facile method to prepare monodispersed Ag/polystyrene composite microspheres and their properties. Polymer 2009, 47: 4547–4547.Google Scholar
- Wen F, Zhang W, Wie G, Wang Y, Zhang J, Zhang M, Shi L: Synthesis of noble metal nanoparticles embedded in the shell layer of core-shell poly(styrene- co -4-vinylpyridine) micospheres and their application in catalysis. Chem Mater 2008, 20: 2144–2150. 10.1021/cm703378cView ArticleGoogle Scholar
- Lu Y, Mei Y, Schrinner M, Ballauff M, Moller MW, Breu J: In situ formation of Ag nanoparticles in spherical polyacrylic acid brushes by UV irradiation. J Phys Chem C 2007, 111: 7676–7681. 10.1021/jp070973mView ArticleGoogle Scholar
- Kim JW, Lee JE, Ryu JH, Lee JS, Kim SJ, Han SH, Chang IS, Kang HH, Suh KD: Synthesis of metal/polymer colloidal composites by the tailored deposition of silver onto porous polymer microspheres. J Polym Sc A 2004, 42: 2551–2554. 10.1002/pola.20125View ArticleGoogle Scholar
- Cuendias A, Backov R, Cloutet E, Cramail H: Synthesis of gold nanoparticles coated onto polyurethane microspheres. J Mater Chem 2005, 15: 4196–4199. 10.1039/b510556kView ArticleGoogle Scholar
- Ou JL, Chang CP, Sung Y, Ou K L, Tseng CC, Ling HW, Ger MD: Uniform polystyrene microspheres decorated with noble metal nanoparticles formed without using extra reducing agent. Colloid Surface A 2007, 305: 36–41. 10.1016/j.colsurfa.2007.04.038View ArticleGoogle Scholar
- Dokoutchaev A, James JT, Koene SC, Pathak S, Prakash GKS, Thompson ME: Colloidal metal deposition onto functionalized polystyrene microsphere. Chem Mater 1999, 11: 2389–2399. 10.1021/cm9900352View ArticleGoogle Scholar
- Jeon SJ, Yang SM, Kim BJ, Petrie JD, Jang SG, Kramer EJ, Pine DJ, Yi GR: Hierarchically structured colloids of diblock copolymers and Au nanoparticles. Chem Mater 2009, 21: 3739–3741. 10.1021/cm9011124View ArticleGoogle Scholar
- Liu W, Yang X, Huang W: Catalytic properties of carboxylic acid functionalized-polymer microsphere-stabilized gold metallic colloids. J Colloid Interf Sci 2006, 304: 160–165. 10.1016/j.jcis.2006.08.040View ArticleGoogle Scholar
- Kohan M: Nylon Plastics Handbook. Cincinnati: Hanser Publishers; 1995.Google Scholar
- Painter PC, Coleman MM: Essentials of Polymer Science and Engineering. Lancaster: Destech Publications; 2008.Google Scholar
- Hvolbaek B, Janssens TVW, Clausen BS, Falsig H, Christensen CH, Norshov JK: Catalytic activity of Au nanoparticles. Nanotodays 2007, 2: 14–18.View ArticleGoogle Scholar
- Jana NR, Wang ZL, Pal T: Redox catalytic properties of palladium nanoparticles: surfactant and electron donor-acceptor effects. Langmuir 2000, 16: 2457–2463. 10.1021/la990507rView ArticleGoogle Scholar
- Mallick K, Witcomb M, Scurrell M: Silver nanoparticle catalysed redox reaction: an electron relay effect. Mater Chem Phys 2006, 97: 283–287. 10.1016/j.matchemphys.2005.08.011View ArticleGoogle Scholar
- Zhou ZY, Kang X, Song Y, Chen S: Butylphenyl-functionalized palladium nanoparticles as effective catalysts for the electro-oxidation of formic acid. Chem Commun 2011, 47: 6075–6077. 10.1039/c1cc11235jView ArticleGoogle Scholar
- Haruta M: Gold catalysts prepared by co-precipitation for low-temperature oxidation of hydrogen and of carbon monoxide. J Cat 1989, 115: 301–309. 10.1016/0021-9517(89)90034-1View ArticleGoogle Scholar
- Mahltig B, Cheval N, Gohy JF, Fahmi A: Preparation of gold nanoparticles under presence of the diblock polyampholyte PMAA-b-PDMAEMA. J Polym Res 2009, 17: 579–588.View ArticleGoogle Scholar
- Chen S, Liu Y, Wu G: Stabilized and size-tunable gold nanoparticles formed in a quaternary ammonium-based room-temperature ionic liquid under gamma-irradiation. Nanotechnology 2005, 16: 2360–2364. 10.1088/0957-4484/16/10/061View ArticleGoogle Scholar
- Fraenkel G, Franconi C: Protonation of amides. J Am Chem Soc 2002, 82: 4478–4483.View ArticleGoogle Scholar
- Sengupta R, Bandyopadhyay A, Sabharwal S, Chaki TK: Polyamide-6,6/ in situ silica hybrid nanocomposites by sol-gel technique: synthesis, characterization and properties. Polymer 2005, 46: 3343–3354. 10.1016/j.polymer.2005.02.104View ArticleGoogle Scholar
- Surovtseva NI, Eremenko AM, Smirnova NP, Pokrovskii VA, Fesenko TV, Starukh GN: The effect of nanosized titania-silica film composition on the photostability of adsorbed methylene blue dye. Theor Exp Chem 2007, 43: 235–240. 10.1007/s11237-007-0027-xView ArticleGoogle Scholar
- Galagan Y, Su WF: Reversible photoreduction of methylene blue in acrylate media containing benzyl dimethyl ketal. J Photoch Photobio A 2008, 195: 378–383. 10.1016/j.jphotochem.2007.11.005View ArticleGoogle Scholar
- Heger D, Jirkovský J, Klán P: Aggregation of methylene blue in frozen aqueous solutions studied by absorption spectroscopy. J Phys Chem A 2005, 109: 6702–6709. 10.1021/jp050439jView ArticleGoogle Scholar
- Rauf MA, Meetani MA, Khaleel A, Ahmed A: Photocatalytic degradation of methylene blue using a mixed catalyst and product analysis by LC/MS. Chem Eng J 2010, 157: 373–378. 10.1016/j.cej.2009.11.017View ArticleGoogle Scholar
- Laoufi I, Lazzari R, Jupille J, Robach O, Garaud S, Cabailh G, Dolle P, Cruguel H, Bailly A: Size and catalytic activity of supported gold nanoparticles: an in operando study during CO oxidation. J Phys Chem C 2011, 115: 4673–4679. 10.1021/jp1110554View ArticleGoogle Scholar
- Jana NR, Pal T: Redox catalytic property of still-growing and final palladium particles: a comparative study. Langmuir 1999, 15: 3458–3463. 10.1021/la981512iView ArticleGoogle Scholar
- Jana NR, Sau TK, Pal T: Growing small silver particle as redox catalyst. J Phys Chem B 1999, 103: 115–121. 10.1021/jp982731fView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.